Balanced infrared nonlinear optical performance achieved by modulating the covalency and ionicity distributions in the electron localization function map.
Liu, Bin-Wen; Jiang, Xiao-Ming; Pei, Shao-Min; Chen, Wen-Fa; Yang, Long-Qi; Guo, Guo-Cong; Materials horizons 8 (2021) 3394–3398; doi:10.1039/d1mh01434j

data_1565092
_publ_section_title
;
 Balanced infrared nonlinear optical performance achieved by modulating
 the covalency and ionicity distributions in the electron localization
 function map.
;
_journal_issue                   12
_journal_name_full               'Materials horizons'
_journal_page_first              3394
_journal_page_last               3398
_journal_paper_doi               10.1039/d1mh01434j
_journal_volume                  8
_journal_year                    2021
_chemical_formula_moiety         Rb2Ba3Li6Ga28S49
_chemical_formula_sum            'Ba3 Ga28 Li6 Rb2 S49'
_chemical_formula_weight         4147.70
_chemical_melting_point          ?
_chemical_name_common            Rb2Ba3Li6Ga28S49
_space_group_IT_number           185
_space_group_name_Hall           'P 6c -2'
_space_group_name_H-M_alt        'P 63 c m'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_H-M   'P 63 c m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_audit_update_record
;
2019-06-17 deposited with the CCDC.	2021-10-08 downloaded from the CCDC.
;
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   19.2355(4)
_cell_length_b                   19.2355(4)
_cell_length_c                   12.0475(4)
_cell_measurement_reflns_used    12993
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      30.9260
_cell_measurement_theta_min      2.7230
_cell_volume                     3860.42(17)
_computing_cell_refinement       'CrysAlisPro 1.171.39.23b (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.39.23b (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.39.23b (Rigaku OD, 2015)'
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 28.5714
_diffrn_measured_fraction_theta_full 0.997
_diffrn_measured_fraction_theta_max 0.997
_diffrn_measurement_device_type  'Rigaku Pilatus CCD'
_diffrn_measurement_method       CCD_Profile_fitting
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0433
_diffrn_reflns_av_sigmaI/netI    0.0307
_diffrn_reflns_limit_h_max       23
_diffrn_reflns_limit_h_min       -23
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            27789
_diffrn_reflns_theta_full        25.49
_diffrn_reflns_theta_max         25.49
_diffrn_reflns_theta_min         3.24
_exptl_absorpt_coefficient_mu    13.679
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.42839
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            colorless
_exptl_crystal_density_diffrn    3.568
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       lamellar
_exptl_crystal_F_000             3824
_exptl_crystal_size_max          0.125
_exptl_crystal_size_mid          0.118
_exptl_crystal_size_min          0.078
_refine_diff_density_max         1.352
_refine_diff_density_min         -0.762
_refine_diff_density_rms         0.094
_refine_ls_abs_structure_details 'Flack H D (1983), Acta Cryst. A39, 876-881'
_refine_ls_abs_structure_Flack   0.006(10)
_refine_ls_extinction_coef       0.000150(9)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.016
_refine_ls_matrix_type           full
_refine_ls_number_parameters     146
_refine_ls_number_reflns         2473
_refine_ls_number_restraints     1
_refine_ls_restrained_S_all      1.016
_refine_ls_R_factor_all          0.0206
_refine_ls_R_factor_gt           0.0180
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0069P)^2^+7.9174P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0426
_refine_ls_wR_factor_ref         0.0435
_reflns_number_gt                2332
_reflns_number_total             2473
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            d1mh01434j2.cif
_cod_data_source_block           Rb2Ba3Li6Ga28S49
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_chemical_melting_point' value 'not measured' was changed
to '?' -- the value is undefined or not given.

data item '_exptl_absorpt_correction_type' value 'Multi-scan' was
changed to 'multi-scan' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_symmetry_cell_setting' value 'Hexagonal' was changed to
'hexagonal' in accordance with the
/home/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

data item '_exptl_crystal_density_meas' value 'not measured' was
changed to '?' -- the value is perceived as not measured.

Automatic conversion script
Id: cif_fix_values 7556 2019-12-06 15:28:31Z antanas 

 Adding full bibliography for 1565090--1565092.cif.
;
_cod_original_sg_symbol_H-M      P63cm
_cod_database_code               1565092